Post weld heat treatment

Short description: Controlled process of reheating materials

Post weld heat treatment (PWHT) is a controlled process in which a material that has been welded is reheated to a temperature below its lower critical transformation temperature, and then it is held at that temperature for a specified amount of time.[1] It is often referred to as being any heat treatment performed after welding; however, within the oil, gas, petrochemical and nuclear industries, it has a specific meaning. Industry codes, such as the ASME Pressure Vessel and Piping Codes, often require mandatory performance of PWHT on certain materials to ensure a safe design with optimal mechanical and metallurgical properties.[2][3]

The need for PWHT is mostly due to the residual stresses and micro-structural changes that occur after welding has been completed.[2] During the welding process, a high temperature gradient is experienced between the weld metal and the parent material. As the weld cools, residual stress is formed.[2] For thicker materials, these stresses can reach an unacceptable level and exceed design stresses. Therefore, the part is heated to a specified temperature for a given amount of time to reduce these stresses to an acceptable level.[1] In addition to residual stresses, microstructural changes occur due to the high temperatures induced by the welding process.[1] These changes can increase hardness of the material and reduce toughness and ductility. The use of PWHT can help reduce any increased hardness levels and improve toughness and ductility to levels acceptable for design.[1]

The requirements specified within various pressure vessels and piping codes are mostly due to the chemical makeup and thickness of the material.[1] Codes such as ASME Section VIII and ASME B31.3 will require that a specified material be post weld heat treated if it is over a given thickness.[1] Codes also require PWHT based solely on the micro-structural make-up of the material.[1] A final consideration in deciding the need for PWHT is based on the components' intended service, such as one with a susceptibility to stress corrosion cracking. In such cases, PWHT is mandatory regardless of thickness.[4]

## Contents

* 1 Application
* 1.1 Heating
* 1.2 Holding temperature and time
* 1.3 Cooling
* 1.4 Monitoring technique
* 2 See also
* 3 References

## Application

Rate of heating, hold times and temperatures, and rate of cooling are all important variables that need to be controlled and monitored precisely, or the desired effects may not be achieved.[3] When PWHT is mandatory by a given industry code, requirements for these variables will be specified.[3][4][5]

### Heating

The rate of heating when PWHT is performed is typically based on the component's thickness and is specified by the governing codes.[1][6]Croft, D (1996). Heat Treatment of Welded Steel Structures. Cambridge England: Woodhead Publishing Ltd. pp. 16-18. ISBN 1-85573-016-2. [7] If the rate of heating is not performed properly, either by heating too quickly or unevenly, temperature gradients within the component can become detrimental to the component. As a result, stress cracks may occur and residual stresses not previously created can form when the component is cooled to ambient temperature.[4]

### Holding temperature and time

Holding temperature and time are governed by the material and thickness respectively.[4][6] Regarding material thickness, longer holding times are needed for thicker materials.[4] This is to allow the material to reach a stable condition where the distribution and levels of stresses become more uniform and decrease.[2][6] The specified holding temperature is one that is at a high enough temperature to relieve high residual stress levels, yet is still below the lower transformation temperature.[1][2] In addition to the reduction of stress, high hold temperatures below the transformation temperature allow for microstructural transformations, therein reducing hardness and improving ductility.[6] Great care should be taken as to not heat the component above the lower transformation temperature, as detrimental metallurgical effects and impaired mechanical properties can result.[6] In addition, the holding temperature should not be greater than the original tempering temperature unless later mechanical testing is performed. Holding above the original tempering temperature can reduce the strength of the material to below ASME required minimums.[4]

### Cooling

As with the heating rate, the cooling rate must be controlled, as to avoid any detrimental temperature gradients that could cause cracking or introduce new stresses during cooling.[4] In addition to this, rapid cooling rates can increase hardness, which may increase the susceptibility of a brittle fracture.[8]

### Monitoring technique

Thermocouples are typically attached to the component undergoing PWHT to check and ensure that heating rates, hold temperatures, and cooling rates meet code specification. Computer software is typically used in conjunction with the thermocouples to monitor the fore-mentioned variables and provide documentation that the PWHT was performed properly.[5][9]

## See also

* Deaerator

## References

1. ↑ 1.0 1.1 1.2 1.3 1.4 1.5 1.6 1.7 1.8 "Post Weld Heat Treatment of Welded Structures". February 2003. http://vibfem.com.au/resources/stress_relieving/post_weld_HT.pdf.
2. ↑ 2.0 2.1 2.2 2.3 2.4 "Heat Treatment of Welded Joints - Part 1". http://www.twi-global.com/technical-knowledge/job-knowledge/heat-treatment-of-welded-joints-part-1-114/.
3. ↑ 3.0 3.1 3.2 Welding Inspection. Miami, FL: American Welding Society. 1980. pp. 38–39. ISBN 978-0-87171-177-9.
4. ↑ 4.0 4.1 4.2 4.3 4.4 4.5 4.6 "Heat treatment of welded joints - Part 2". http://www.twi-global.com/technical-knowledge/job-knowledge/heat-treatment-of-welded-joints-part-2-115/.
5. ↑ 5.0 5.1 "Heat Treatment Part 3". http://www.twi-global.com/technical-knowledge/job-knowledge/heat-treatment-of-welded-joints-part-3-116/.
6. ↑ 6.0 6.1 6.2 6.3 6.4 Croft, D (1996). Heat Treatment of Welded Steel Structures. Cambridge England: Woodhead Publishing Ltd. pp. 16–18. ISBN 1-85573-016-2.
7. ↑ See more at <a href="https://www.hgcmanchester.com/post-welding-heat-treatment-material/" target="_blank">Post Welding Heat Treatment Material</a>
8. ↑ Thielsch, Helmut (1977). Defects and Failures in Pressure Vessels and Piping. Malabar, Florida: Krieger Publishing Company. pp. 305. ISBN 978-0-88275-308-9.
9. ↑ "Weld Heat Treatment". https://axiomht.com/.

* v
* t
* e

Iron and steel production

* History of ferrous metallurgy
* List of steel producers

Iron production
(Ironworks)|

| Smelting|

* Bloomery (produces sponge iron)
* Blast furnace (produces pig iron)
* Cold blast
* Hot blast
* Anthracite iron
* Direct reduced iron

|

Secondary|

* Wrought iron (via Finery forge or Reverberatory Puddling Furnace)
* Cast iron (via Cupola furnace or Induction furnace)

Steelmaking
(Steel mill)|

| Primary (Pre-1850)|

* Pattern welding
* Crucible steel (Damascus steel)
* Tatara furnace
* Cementation process

|

Primary (Post-1850)|

* Bessemer process
* Open hearth furnace
* Electric arc furnace
* Basic oxygen process

Secondary|

* Electro-slag remelting
* Vacuum arc remelting
* Argon oxygen decarburization

Production by country|

* Bangladesh
* China
* India
* Italy
* Luxembourg
* United States

Heat treatment methods|

| Annealing|

* Low hydrogen
* Short circuit

|

Hardening /
Case-hardening|

* Ausforming
* Boriding
* Carbonitriding
* Carburizing
* Cryogenic
* Ferritic nitrocarburizing
* Induction
* Nitriding
* Precipitation
* Quench polish quench

Tempering|

* Austempering
* Martempering

* Cryogenic treatment (Deburring
* Deflashing
* Hardening)
* Differential heat treatment
* Decarburization
* Forming gas
* Post weld heat treatment
* Quenching
* Superplastic forming

0.00

(0 votes)

Original source: https://en.wikipedia.org/wiki/Post weld heat treatment. Read more

|

Retrieved from "https://handwiki.org/wiki/index.php?title=Engineering:Post_weld_heat_treatment&oldid=3874131"
*[v]: View this template
*[t]: Discuss this template
*[e]: Edit this template